hydration products of portland cementWojciech Franus
Division of Geotechnics, Lublin University of Technology, Nadbystrzycka 40, 20-618 Lublin, Poland, E-mail: firstname.lastname@example.org
Division of Geotechnics, Lublin University of Technology, Nadbystrzycka 40, 20-618 Lublin, Poland, E-mail: email@example.com
Mineral and Energy Economy Research Institute of the Polish Academy of Sciences, Wybickiego 7, 31-261 Kraków, Poland, E-mail: firstname.lastname@example.org
Abstract Portland cement is the one of the main ingredients in the manufacture of many building materials include concrete composites. The phase composition of hydration products is controlled by means of XRD and DTA/TG analysis. Obser-vations of phase changes and microstructure of maturing cement pastes can also be observed using scanning electron microscopy (SEM) techniques combined with chemical analyzes in microareas (EDS analysis). Hydrating in time cement paste is composed mainly of hydrated silicates of calcium so called C-S-H-phase ac-companied with a calcium hydroxide (portlandite) and hydration products of cal-cium aluminate i.e. ettringite. SEM analysis of changes in the morphology and microstructure of cement pastes allow to track the hydration progress observed mainly by changes in the C-S-H phase. The initial stages of hydration of this phase is characterized by radial concentration of fibers or needles, often narrowed at the ends. This fibers grow from the surface of the cement grains. The increase in the degree of C-S-H structure orientation is shown by formation of fibers lat-tice, sometimes three-dimensional plates so called "honeycomb", which is trans-formed into the form of a closely-packed, isometric grains. In addition, besides C-S-H cement phase investigation, scanning electron microscopy can also be applied to observation of the crystals formation of tobermorite, ettringite and relicts of portlandite, that often can’t be detected by XRD and DTA/TG due to their small amount in mineral composition of concrete.
Knowledge of the basic chemical reactions and physical phenomena as well as microstructures of the hardened mass formed by the hydration and hydrolysis of cement is one of the basic conditions for the optimal use of cement in building materials. Predicting the cement properties on the basis of its chemical and miner-al composition is essentiminer-al for its use . No fully define mechanism of the ce-ment hydration and hydrolysis processes does not allow for explanation anomalies in the process of binding and hardening. Strength of hardened cement paste is a function of: mineral and chemical composition as well as has a direct impact on the structure that determines the strength of the crystalline lattice and tightness of mass. Therefore, they are needed studies of crystallizing mineral phases changes (hydration products) and observations of the reconstruction of the microstructure of maturing cement paste . Method used to determine this type of phenomena may be scanning electron microscopy combined with the chemical composition analysis (SEM-EDS).
Quantitatively, the main component of the most cement paste and at the same time the most important factor affecting the strength of the hardening mass is phase denoted by the symbol C-S-H - often called phase of tobermorite-like or tobermorite because its chemical composition is similar to natural mineral - tobermorite (5CaO·6SiO2·5H2O). This phase in general is the entire group of
com-pounds of a hydrated calcium silicate with varying degrees of crystallization and differential alkalinity. The hydration and hardening mechanisms of cement is based on density of C-S-H gel combined with the addition of water and crystalli-zation of ettringite and calcium hydroxide intergrowths forming and filling pores in hardening cement paste. Knowledge of the mineral composition and structure during maturation cement paste allow to predict its technical properties .
The hydration process of cement pastes were observed on the basis of mortars samples prepared in accordance with PN-EN 196-1: 1996. To this aim bars about size of 40x40x160 mm were done, the composition of which was as follows: Port-land cement CEM I 42.5 R (450 g), standard sand (1350 g), water (225 g). Thus formed samples were aged in water and subjected to observation of changes in the phase composition with SEM after 2, 28 and 90 days of maturing.
The chemical and mineral composition of products hydration were deter-mined by using a scanning electron microscope SEM–EDS and X-ray method. The morphological forms and the chemical composition of the main mineral com-ponents were analysing by means of a scanning electron microscope (SEM) FEI Quanta 250 FEG equipped with a system of chemical composition analysis based on energy dispersive X-ray- EDS of EDAX company .
The mineral composition was determined via powder X-ray diffraction (XRD) method using a Philips X’pert APD diffractometer (with a PW 3020 goni-ometer), Cu lamp, and a graphite monochromator. The analysis was performed within the angle range of 5–65 2 theta. Philips X’Pert Highscore software was used to process the diffraction data. The identification of mineral phases was based on the PDF-2 release 2010 database formalized by the ICDD .
4. RESULTS AND DISCUSSION
The hydration process of cement and development of cement paste structure can be presented in three stages, depicted in Figure 4.1.
In the first stage of cement hydration the calcium hydroxide (portlandite) is separated. Its formation is a result of the hydrolysis of tricalcium (C3S) and
dicalcium (C2S) silicates, what has a place after a few hours of mixing Portland
cement with water. The resulting calcium hydroxide at solid phase of paste is pre-sent primarily in the form of portlandite. It creates massive, hexagonal crystals about size of 40 microns (Fig. 4.2), which aggregates taking the form of column (Fig. 4.3). The morphology of the resulting portlandite crystals is dependent on available free space for crystallization (w/c), the type of admixtures and additives . Portlandite in hydratated paste of Portland cement is up to 25% by volume of solid phase.
Fig.4.2 Hexagonal plate of portlandite Fig.4.3 Column aggregate of portlandite
Fig.4.4 Needle form of C-S-H and plates of portlandite
Fig.4.5 Transformations of portlandite into solid forms, and needle forms of C-S-H into “honeycomb” structure
In the second period of hydration of cement paste the first forms of hydrated calcium silicates are created. Their quantitative contents in completely hydrated paste of Portland cement is between 50-60% of the volume of all solid phases.
Proposed by Diamond  model of the morphological distribution of C-S-H gel in cement paste distinguish form of fiber from size of 2 microns - characteristic for the early stages of hydration (Fig. 4.4), which goes in the form of a mesh, so-called "honeycomb" (Fig. 4.5). Subsequent stages of maturing the paste constitut-ed forms becoming more and more massive consisting of a packconstitut-ed and inter-spersed with each other thin crystals (so called foils), up to the formless and mas-sive gel characteristic for old pastes.
In the third period of paste hydration occurs pore filling of hardening cement paste by short fibers or lamellar phases of hydrated calcium silicates. The duration of this stages is a period of several days to several months, and covers almost complete hydration of the cement. A characteristic feature of this phase is trans-formation of calcium aluminate trisulfate 3CaO·Al2O3·3CaSO4·32 H2O to calcium
aluminate monosulfate 3CaO·Al2O3·CaSO4·12 H2O. Ettringite crystals and AFt
phases typically form an elongated crystals about circular habit similar to the nee-dle (Figure 4.7.), while tobermorite create lamellar aggregates (Fig. 4.8). The spectra of the chemical composition of the main phase formed during the matura-tion of the cement paste is shown in figure 4.6.
EDS of C-S-H phase EDS of portlandite EDS of C-S-H honeycomb
Fig.4.6 Mineral phases occurring in maturing cement paste.
Scanning microscope observations also allow to identify the minerals forming the relics of clinker for example periclase that the presence in the paste in the form of large crystals unfavorably affects the stability of the structure of maturing ce-ment pastes (Fig. 4.9). These types of mineral phases due to their trace amounts in tested samples are not recognizable by diffraction (XRD), or thermal (TG-DTA) methods.
Fig.4.7Needle crystals of ettringite
Fig.4.8 plate crystals of tobemorite
Fig.4.9 Octahedral forms of periclase
The presented results obtained by means of scanning electron microscopy with chemical microanalysis (SEM-EDS) indicate the practical opportunity to observe changes in the microstructure of maturing cement pastes or concrete. Based on changes in the morphology of the main phases arising during the hydration of ce-ment paste it is possible to predict the properties of cece-ment mortars and concretes.
Acknowledgments This research was financed by PL-BY-UA within the Project No IPBU.01.01.00-06-570/11-00 and Operational Program within the Project No POKL.04.03.00-00-129/12
1. HansenT. C., Physical structure of hardened cement paste. A classical approach Materials and Structures, Volume 19, Issue 6, pp 423-436 (1986)
2. Arandigoyen M., AlvarezJ.I., Pore structure and mechanical properties of cement–lime mor-tars. Cement and Concrete Research Volume 37, Issue 5, Pages 767–775 (2007)
3. Kurdowski W., Chemia cementu i betonu. pp. 1-727 Wyd. PWN, (2010)
4. Wdowin M., Franus M., Panek R., Bandura L., Franus W., The conversion technology of fly ash into zeolites. Clean Technologies and Environmental Policy.16:1217-1223 (2014) 5. Franus W, Dudek K., Clay minerals and clinoptilolite of Variegated Shales Formation of the
Skole Unit. Polish Fly Asch Carpathians. Geologica Carpathica, vol. 50, p. 23-24 (1999) 6. Locher R., Richartz W., Study of hydration mechanism of cement. Symp. Chem. Cement
Moscow, Moscow, Russia (1974)
7. Mehta P.K., Concrete, structure, properties and materials. Englewood Cliffs, NJ, Prentice-Hall, pp. 450, (1986)
9. Diamond S., The Microstructures of cement paste in concrete, 8th ICCCC. Vol. 1 pp. 113-121, Rio de Janeiro (1986)